Download presentation

Presentation is loading. Please wait.

Published byUlysses Peers Modified about 1 year ago

1
MECHANICS OF MATERIALS Third Edition Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University CHAPTER © 2002 The McGraw-Hill Companies, Inc. All rights reserved. 2 Stress and Strain – Axial Loading

2
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 2 Contents Stress & Strain: Axial Loading Normal Strain Stress-Strain Test Stress-Strain Diagram: Ductile Materials Stress-Strain Diagram: Brittle Materials Hooke’s Law: Modulus of Elasticity Elastic vs. Plastic Behavior Fatigue Deformations Under Axial Loading Example 2.01 Sample Problem 2.1 Static Indeterminacy Example 2.04 Thermal Stresses Poisson’s Ratio Generalized Hooke’s Law Dilatation: Bulk Modulus Shearing Strain Example 2.10 Relation Among E,, and G Sample Problem 2.5 Composite Materials Saint-Venant’s Principle Stress Concentration: Hole Stress Concentration: Fillet Example 2.12 Elastoplastic Materials Plastic Deformations Residual Stresses Example 2.14, 2.15, 2.16

3
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 3 Stress & Strain: Axial Loading Suitability of a structure or machine may depend on the deformations in the structure as well as the stresses induced under loading. Statics analyses alone are not sufficient. Considering structures as deformable allows determination of member forces and reactions which are statically indeterminate. Determination of the stress distribution within a member also requires consideration of deformations in the member. Chapter 2 is concerned with deformation of a structural member under axial loading. Later chapters will deal with torsional and pure bending loads.

4
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 4 Normal Strain

5
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 5 Stress-Strain Test

6
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 6 Stress-Strain Diagram: Ductile Materials

7
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 7 Stress-Strain Diagram: Brittle Materials

8
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 8 Hooke’s Law: Modulus of Elasticity Below the yield stress Strength is affected by alloying, heat treating, and manufacturing process but stiffness (Modulus of Elasticity) is not.

9
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 9 Elastic vs. Plastic Behavior If the strain disappears when the stress is removed, the material is said to behave elastically. When the strain does not return to zero after the stress is removed, the material is said to behave plastically. The largest stress for which this occurs is called the elastic limit.

10
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 10 Fatigue Fatigue properties are shown on S-N diagrams. When the stress is reduced below the endurance limit, fatigue failures do not occur for any number of cycles. A member may fail due to fatigue at stress levels significantly below the ultimate strength if subjected to many loading cycles.

11
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 11 Deformations Under Axial Loading From Hooke’s Law: From the definition of strain: Equating and solving for the deformation, With variations in loading, cross-section or material properties,

12
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 12 Example 2.01 Determine the deformation of the steel rod shown under the given loads. SOLUTION: Divide the rod into components at the load application points. Apply a free-body analysis on each component to determine the internal force Evaluate the total of the component deflections.

13
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 13 SOLUTION: Divide the rod into three components: Apply free-body analysis to each component to determine internal forces, Evaluate total deflection,

14
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 14 Sample Problem 2.1 The rigid bar BDE is supported by two links AB and CD. Link AB is made of aluminum (E = 70 GPa) and has a cross-sectional area of 500 mm 2. Link CD is made of steel (E = 200 GPa) and has a cross-sectional area of (600 mm 2 ). For the 30-kN force shown, determine the deflection a) of B, b) of D, and c) of E. SOLUTION: Apply a free-body analysis to the bar BDE to find the forces exerted by links AB and DC. Evaluate the deformation of links AB and DC or the displacements of B and D. Work out the geometry to find the deflection at E given the deflections at B and D.

15
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 15 Displacement of B: Displacement of D: Free body: Bar BDE SOLUTION: Sample Problem 2.1

16
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 16 Displacement of D: Sample Problem 2.1

17
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 17 Static Indeterminacy Structures for which internal forces and reactions cannot be determined from statics alone are said to be statically indeterminate. Deformations due to actual loads and redundant reactions are determined separately and then added or superposed. Redundant reactions are replaced with unknown loads which along with the other loads must produce compatible deformations. A structure will be statically indeterminate whenever it is held by more supports than are required to maintain its equilibrium.

18
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 18 Example 2.04 Determine the reactions at A and B for the steel bar and loading shown, assuming a close fit at both supports before the loads are applied. Solve for the reaction at A due to applied loads and the reaction found at B. Require that the displacements due to the loads and due to the redundant reaction be compatible, i.e., require that their sum be zero. Solve for the displacement at B due to the redundant reaction at B. SOLUTION: Consider the reaction at B as redundant, release the bar from that support, and solve for the displacement at B due to the applied loads.

19
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 19 SOLUTION: Solve for the displacement at B due to the applied loads with the redundant constraint released, Solve for the displacement at B due to the redundant constraint, Example 2.04

20
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 20 Require that the displacements due to the loads and due to the redundant reaction be compatible, Find the reaction at A due to the loads and the reaction at B Example 2.04

21
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 21 Thermal Stresses A temperature change results in a change in length or thermal strain. There is no stress associated with the thermal strain unless the elongation is restrained by the supports. Treat the additional support as redundant and apply the principle of superposition. The thermal deformation and the deformation from the redundant support must be compatible.

22
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 22 Poisson’s Ratio For a slender bar subjected to axial loading: The elongation in the x-direction is accompanied by a contraction in the other directions. Assuming that the material is isotropic (no directional dependence), Poisson’s ratio is defined as

23
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 23 Generalized Hooke’s Law For an element subjected to multi-axial loading, the normal strain components resulting from the stress components may be determined from the principle of superposition. This requires: 1)strain is linearly related to stress 2)deformations are small With these restrictions:

24
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf Dilatation: Bulk Modulus Relative to the unstressed state, the change in volume is For element subjected to uniform hydrostatic pressure, Subjected to uniform pressure, dilatation must be negative, therefore

25
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 25 Shearing Strain A cubic element subjected to a shear stress will deform into a rhomboid. The corresponding shear strain is quantified in terms of the change in angle between the sides, A plot of shear stress vs. shear strain is similar the previous plots of normal stress vs. normal strain except that the strength values are approximately half. For small strains, where G is the modulus of rigidity or shear modulus.

26
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 26 Example 2.10 A rectangular block of material with modulus of rigidity G = 90 ksi is bonded to two rigid horizontal plates. The lower plate is fixed, while the upper plate is subjected to a horizontal force P. Knowing that the upper plate moves through 0.04 in. under the action of the force, determine a) the average shearing strain in the material, and b) the force P exerted on the plate. SOLUTION: Determine the average angular deformation or shearing strain of the block. Use the definition of shearing stress to find the force P. Apply Hooke’s law for shearing stress and strain to find the corresponding shearing stress.

27
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 27 Determine the average angular deformation or shearing strain of the block. Apply Hooke’s law for shearing stress and strain to find the corresponding shearing stress. Use the definition of shearing stress to find the force P.

28
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 28 Relation Among E, and G An axially loaded slender bar will elongate in the axial direction and contract in the transverse directions. Components of normal and shear strain are related, If the cubic element is oriented as in the bottom figure, it will deform into a rhombus. Axial load also results in a shear strain. An initially cubic element oriented as in top figure will deform into a rectangular parallelepiped. The axial load produces a normal strain.

29
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 29 Sample Problem 2.5 A circle of diameter d = 9 in. is scribed on an unstressed aluminum plate of thickness t = 3/4 in. Forces acting in the plane of the plate later cause normal stresses x = 12 ksi and z = 20 ksi. For E = 10x10 6 psi and = 1/3, determine the change in: a)the length of diameter AB, b)the length of diameter CD, c)the thickness of the plate, and d)the volume of the plate.

30
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 30 SOLUTION: Apply the generalized Hooke’s Law to find the three components of normal strain. Evaluate the deformation components. Find the change in volume

31
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 31 Composite Materials Fiber-reinforced composite materials are formed from lamina of fibers of graphite, glass, or polymers embedded in a resin matrix. Normal stresses and strains are related by Hooke’s Law but with directionally dependent moduli of elasticity, Transverse contractions are related by directionally dependent values of Poisson’s ratio, e.g., Materials with directionally dependent mechanical properties are anisotropic.

32
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 32 Saint-Venant’s Principle Loads transmitted through rigid plates result in uniform distribution of stress and strain. Saint-Venant’s Principle: Stress distribution may be assumed independent of the mode of load application except in the immediate vicinity of load application points. Stress and strain distributions become uniform at a relatively short distance from the load application points. Concentrated loads result in large stresses in the vicinity of the load application point.

33
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 33 Stress Concentration: Hole Discontinuities of cross section may result in high localized or concentrated stresses.

34
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 34 Stress Concentration: Fillet

35
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 35 Example 2.12 Determine the largest axial load P that can be safely supported by a flat steel bar consisting of two portions, both 10 mm thick, and respectively 40 and 60 mm wide, connected by fillets of radius r = 8 mm. Assume an allowable normal stress of 165 MPa. SOLUTION: Determine the geometric ratios and find the stress concentration factor from Fig. 2.64b. Apply the definition of normal stress to find the allowable load. Find the allowable average normal stress using the material allowable normal stress and the stress concentration factor.

36
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 36 Determine the geometric ratios and find the stress concentration factor from Fig. 2.64b. Find the allowable average normal stress using the material allowable normal stress and the stress concentration factor. Apply the definition of normal stress to find the allowable load.

37
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 37 Elastoplastic Materials Previous analyses based on assumption of linear stress-strain relationship, i.e., stresses below the yield stress Assumption is good for brittle material which rupture without yielding If the yield stress of ductile materials is exceeded, then plastic deformations occur Analysis of plastic deformations is simplified by assuming an idealized elastoplastic material Deformations of an elastoplastic material are divided into elastic and plastic ranges Permanent deformations result from loading beyond the yield stress

38
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 38 Plastic Deformations Elastic deformation while maximum stress is less than yield stress Maximum stress is equal to the yield stress at the maximum elastic loading At loadings above the maximum elastic load, a region of plastic deformations develop near the hole As the loading increases, the plastic region expands until the section is at a uniform stress equal to the yield stress

39
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 39 Residual Stresses When a single structural element is loaded uniformly beyond its yield stress and then unloaded, it is permanently deformed but all stresses disappear. This is not the general result. Residual stresses also result from the uneven heating or cooling of structures or structural elements Residual stresses will remain in a structure after loading and unloading if -only part of the structure undergoes plastic deformation -different parts of the structure undergo different plastic deformations

40
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 40 Example 2.14, 2.15, 2.16 A cylindrical rod is placed inside a tube of the same length. The ends of the rod and tube are attached to a rigid support on one side and a rigid plate on the other. The load on the rod-tube assembly is increased from zero to 5.7 kips and decreased back to zero. a)draw a load-deflection diagram for the rod-tube assembly b)determine the maximum elongation c)determine the permanent set d)calculate the residual stresses in the rod and tube.

41
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 41 a)draw a load-deflection diagram for the rod- tube assembly Example 2.14, 2.15, 2.16

42
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 42 b,c) determine the maximum elongation and permanent set at a load of P = 5.7 kips, the rod has reached the plastic range while the tube is still in the elastic range the rod-tube assembly unloads along a line parallel to 0Y r Example 2.14, 2.15, 2.16

43
© 2002 The McGraw-Hill Companies, Inc. All rights reserved. MECHANICS OF MATERIALS ThirdEdition Beer Johnston DeWolf 2 - 43 calculate the residual stresses in the rod and tube. calculate the reverse stresses in the rod and tube caused by unloading and add them to the maximum stresses. Example 2.14, 2.15, 2.16

Similar presentations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google